Abstract
Atomic manipulation techniques have provided a bottomup approach to investigating the unconventional properties and complex phases of strongly correlated electron materials. By engineering artificial systems containing tens to thousands of atoms with tailored electronic or magnetic properties, it has become possible to explore how quantum manybody effects emerge as the size of a system is increased from the nanoscale to the mesoscale. Here we investigate both theoretically and experimentally the quantum engineering of nanoscale Kondo lattices – Kondo droplets – exemplifying nanoscopic replicas of heavyfermion materials. We demonstrate that by changing a droplet’s realspace geometry, we can not only create coherently coupled Kondo droplets whose properties asymptotically approach those of a quantumcoherent Kondo lattice, but also markedly increase or decrease the droplet’s Kondo temperature. Furthermore we report on the discovery of a new quantum phenomenon – the Kondo echo – a signature of droplets containing Kondo holes functioning as direct probes of spatially extended, quantumcoherent Kondo cloud correlations.
Introduction
Quantum engineering of finitesize artificial adatom lattices^{1,2,3,4,5,6,7} on metallic surfaces has provided a unique approach to explore how variations in the lattice shape or structure affect emergent electronic properties. This has given rise to the creation of Dirac cones in molecular graphene^{5} and artificial Lieb lattices^{6}, as well as the discovery of many quantum phenomena, such as quantum mirages in Kondo corrals^{1,2} or topological superconductivity^{7}. Artificial lattices also open a new road to studying the emergence of strong correlation effects^{8,9,10,11,12} through the use of magnetic adatoms, and the ensuing Kondo effect^{13}. Such Kondo lattices^{4}, which when rendered coherent, are believed to contain all salient features of heavyfermion materials. They should permit the exploration of how manybody phenomena emerge at the nanoscale, evolve across the mesoscale, and result in the many complex properties of macroscopic systems^{14}. At the same time, atomic manipulation techniques enable the controlled implementation of defects or vacancies, opening up a new field for studying the interplay between disorder and strong correlation effects. These possibilities might hold the key to greatly advancing our understanding of the many unconventional properties and complex phases of strongly correlated electron materials at the macroscale^{9,10}.
In the following, we demonstrate theoretically and experimentally how the properties of Kondo droplets are affected by the droplet’s realspace geometry and evolve with increasing droplet size. In particular, we show that by changing a droplet’s realspace geometry, we can (a) quantum engineer coherently coupled Kondo droplets whose properties asymptotically approach those of a quantumcoherent Kondo lattice, and (b) markedly increase or decrease the droplet’s Kondo temperature. As these coherent Kondo droplets can be created with fewer than 50 adatoms, our results open an arena for the exploration of heavyfermion physics at the nanoscale. Furthermore, we demonstrate that a Kondo echo emerges at Kondo hole sites in a Kondo droplet as a characteristic signature of spatially extended, quantumcoherent Kondo cloud correlations.
Results
LargeN theory for Kondo droplets
To study the emergence of correlation effects in Kondo droplets, we use atomic manipulation to arrange magnetic Co adatoms on metallic Cu(111) surfaces^{1} in the form of highly ordered, hexagonal Kondo droplets (Fig. 1a–d). After benchmarking the intact lattices, we study defects in the form of Kondo holes created through missing Co adatoms (Fig. 1e). Cu(111) surfaces are uniquely suited to investigate the emergence of manybody effects in Kondo droplets, as Kondo screening arises from the coupling to a surface band of twodimensional electrons^{1}—in which correlation effects are expected to be spatially longer ranged—rather than to threedimensional bulk bands. Such Kondo droplets are described by the Kondo Hamiltonian^{8,13,15,16,17,18,19,20}
where \({c}_{{\bf{r}},\sigma }^{\dagger }\)\(({c}_{{\bf{r}},\sigma })\) creates (annihilates) a conduction electron with spin \(\sigma\) at site \({\bf{r}}\) on the Cu surface. Here, \({t}_{{\bf{r}}{\bf{r}}^{\prime} }=0.924\) eV is the fermionic hopping element between nearestneighbor sites in the triangular Cu(111) surface lattice, and \(\mu =5.13\) eV is its chemical potential, yielding a Fermi wavelength of \({\lambda }_{{\rm{F}}}\approx 11.5{a}_{0}\), where \({a}_{0}\) is the Cu lattice constant^{2,5}. Moreover, \(J\, > \, 0\) is the Kondo coupling, and \({{\bf{S}}}_{{\bf{r}}}^{{\rm{K}}}\) and \({{\bf{s}}}_{{\bf{r}}}^{{\rm{c}}}\) are the spin operators of the magnetic Co adatom and the conduction electron at site \({\bf{r}}\), respectively. The primed sum runs over the locations of the Co adatoms only. We note that the lattice structure of the Cu(111) surface allows for the creation of two natural types of hexagonal Kondo droplets (which are rotated by \(3{0}^{\circ }\) with respect to each other) with adatom distances of \(\Delta {r}_{{\rm{1}}}=n{a}_{0}\) (see Fig. 2a) and \(\Delta {r}_{{\rm{2}}}=n\sqrt{3}{a}_{0}\) (see Fig. 2b) with \(n\) being an integer.
To describe the Kondo screening of the Co adatoms by Cu(111) surface electrons, we employ a largeN expansion^{15,16,17,20,21,22,23}, which has previously been used to successfully explain^{24,25} the asymmetric form of the Kondo resonance in the differential conductance, \({\mathrm{d}}I/{\mathrm{d}}V\), measured via scanning tunneling spectroscopy (STS). Here, \({{\bf{S}}}_{{\bf{r}}}^{{\rm{K}}}\) is generalized to \(SU(N)\) and represented via Abrikosov pseudofermion operators \({f}_{{\bf{r}},\alpha }^{\dagger },{f}_{{\bf{r}},\alpha }\), which obey the constraint \({\sum }_{\alpha =1..N}{f}_{{\bf{r}},\alpha }^{\dagger }{f}_{{\bf{r}},\alpha }=1\) with \(N=2S+1\) being the spin degeneracy of the magnetic adatom. This constraint is enforced at every site of the Kondo droplet by means of a Lagrange multiplier \({\varepsilon }_{{\rm{f}}}({\bf{r}})\), while the exchange interaction in Eq. (1) is decoupled via a hybridization field, \(s({\bf{r}})\). The hybridization represents the hopping amplitude between the conduction electron states and the pseudofermion \(f\)electron states and reflects the strength of the Kondo screening. In particular, for a single Kondo impurity, the onset temperature for Kondo screening, the Kondo temperature \({T}_{{\rm{K}}}\), is related to the width of the Kondo resonance, \(\Delta {E}_{{\rm{K}}}\), in the differential conductance (see below) via \({k}_{\rm{B}}{T}_{{\rm{K}}}=\Delta {E}_{{\rm{K}}}\), with the latter scaling as \(\Delta {E}_{{\rm{K}}} \sim {s}^{2}\) (see ref. ^{16}). For fixed \(J\), \({\varepsilon }_{{\rm{f}}}({\bf{r}})\) and \(s({\bf{r}})\) are obtained on the saddle point level by minimizing the effective action^{21} [for details see Supplementary Note 1]. We note that the Ruderman–Kittel–Kasuya–Yosida (RKKY) interaction between magnetic moments^{8,16,19} for the twodimensional (2D) Cu(111) surface band decays rapidly with increasing distance^{26}, and is significantly smaller than \({k}_{\rm{B}}{T}_{{\rm{K}}}\) for the relevant interadatom distances considered below, in agreement with experimental findings^{27}, such that this interaction can be neglected. Finally, to reproduce the lineshape and width of the Kondo resonance measured experimentally^{1} for a single Co adatom on a Cu(111) surface, we employ \(J=3.82\) eV and \(N=4\) (see below and ref. ^{24}).
Evolution of Kondo screening with increasing droplet size
To investigate the evolution of Kondo screening from a single Kondo impurity to the Kondo lattice, we begin by considering how the droplet’s physical properties change with increasing number of rings of Co adatoms with adatom distance \(\Delta {r}_{{\rm{2}}}=4\sqrt{3}{a}_{0}\) (see Fig. 2b). To this end, we present in Fig. 2c the selfconsistently computed hybridization, \(s({\bf{r}})\), for different adatom sites in the Kondo droplet (as denoted in Fig. 2b) and increasing number of adatom rings. A key physical fact that emerges is that the hybridization in the center of the droplet—denoted as site \(p=0\)—decreases with increasing number of rings, with the decreasing rate of change between consecutive rings indicating that it approaches an asymptotic value. As the hybridization for a single Kondo adatom is in general larger than that for a Kondo lattice (assuming the same set of parameters) – essentially since the conduction electrons take part in the Kondo screening of multiple magnetic adatoms – this decrease of \(s\) with increasing droplet size reflects the crossover in the droplet’s properties from those of a single Kondo impurity to those of a Kondo lattice. Moreover, as one moves from the droplet’s center to its edge, the hybridization increases, indicating that the properties of the Kondo adatoms along the edge lie between those of the bulk (as exemplified by the droplet’s center) and those of a single Kondo impurity. In Fig. 2d, e, we present a spatial plot of \(s({\bf{r}})\) and of the width of the Kondo resonance, \(\Delta {E}_{{\rm{K}}}({\bf{r}})\), at the site of the Co adatoms, respectively, for a Kondo droplet with three rings of magnetic adatoms [\(\Delta {E}_{{\rm{K}}}({\bf{r}})\) is extracted by fitting the Fano formula^{28} to the theoretical \({\mathrm{d}}I/{\mathrm{d}}V\) lineshape, as described in Supplementary Note 2]. It is intriguing that these two properties are anticorrelated: while \(s({\bf{r}})\) is smaller in the center of the droplet than at the edge (for the reasons discussed above), \(\Delta {E}_{{\rm{K}}}({\bf{r}})\) is larger in the center. Indeed, the larger value of \(\Delta {E}_{{\rm{K}}}({\bf{r}})\) in the center, reflecting the coherent coupling of individual Kondo resonances, is another signature of the crossover to a Kondo lattice: with increasing number of rings, the suppression of the density of states in the Kondo resonance becomes larger and more extended in energy as it evolves into the hybridization gap^{29}. The anticorrelated spatial structure of \(s({\bf{r}})\) and \(\Delta {E}_{{\rm{K}}}({\bf{r}})\) shown in Fig. 2d, e, therefore, directly reflect the different physical properties of a Kondo impurity and a Kondo lattice. These results thus imply that it is possible to study the crossover from a single Kondo impurity to the Kondo lattices not only with increasing droplet size, but also within the same droplet exhibiting bulk properties in its center and properties more similar to isolated impurities along its edges.
Quantumcoherent and incoherent Kondo droplets
The hybridization as well as the width of the Kondo resonance, \(\Delta {E}_{{\rm{K}}}\), can be controlled in a nonmonotonic fashion, by varying the distance between the magnetic adatoms, \(\Delta r\). To demonstrate this, we present in Fig. 3a the width of the Kondo resonance, \(\Delta {E}_{{\rm{K}}}({\bf{r}})\) (see Supplementary Note 2), at the center and edge sites (the latter denoted as site \(p=3\) in Fig. 2b) of a Kondo droplet with three rings for increasing interadatom distance. Not only is the dependence of \(\Delta {E}_{{\rm{K}}}\) on \(\Delta r\) nonmonotonic, but \(\Delta {E}_{{\rm{K}}}\) can also be significantly enhanced or suppressed from that of a single Kondo impurity (thick blue line), with the largest enhancement and suppression at the center site occurring for \(\Delta r=4\sqrt{3}{a}_{0}\) and \(\Delta r=3{a}_{0}\), respectively. The large difference in \(\Delta {E}_{{\rm{K}}}\) for these two Kondo droplets is clearly revealed in the \({\rm{d}}I/{\rm{d}}V\) lineshape at the center sites, shown in Fig. 3b. This nonmonotonic behavior of \(\Delta {E}_{{\rm{K}}}\) arises from the constructive or destructive quantum interference between the Kondo screening clouds associated with each individual magnetic adatom (Fig. 1e and Supplementary Note 3). We note that with increasing droplet size, the width of the Kondo resonance increases and evolves into the hybridization gap of the coherent Kondo lattice^{29}. As such, the increased \(\Delta {E}_{{\rm{K}}}\) for \(\Delta r=4\sqrt{3}{a}_{0}\) is strong evidence for the coherent and constructive coupling of the Kondo screening clouds associated with the individual magnetic adatoms, and hence the creation of a coherent Kondo droplet hosting extended Kondo cloud correlations. On the other hand, for \(\Delta r=3{a}_{0}\) the Kondo resonance at the center of the droplet is strongly suppressed, indicating the destructive interference of the Kondo screening clouds. This demonstrates that the creation of a coherent, nanoscale Kondo lattice can be controlled through manipulation of the droplet’s geometry and the ensuing quantum interference processes.
Experimentally engineered Kondo droplets
While our theoretical results predict the largest difference in the strength of the Kondo screening between droplets with \(\Delta r=4\sqrt{3}{a}_{0}\) and \(\Delta r=3{a}_{0}\), we find experimentally that Co lattices with \(n \, < \, 4\) are insufficiently stable for detailed spectroscopy. On the other hand, for the two lattice types shown in Fig. 2a, b, the \(n=4\) family yields nearestneighbor magnetic moment distances closest to and straddling \({\lambda }_{F}/2 \sim 15\) Å, corresponding to the screening limit of \(\sim \!\!1\) itinerant electron per spin impurity. Moreover, our theoretical results predict a large difference in correlated behavior between the two types of \(n=4\) droplets (Fig. 3a), contrasting a nearly uncorrelated droplet (dashed vertical black arrow) with a maximally coherent state (solid vertical black arrow). Accordingly, we use atomic manipulation techniques to build two Kondo droplets, each consisting of three rings of Co adatoms with adatom distances of \(\Delta {r}_{{\rm{1}}}=4{a}_{0}\approx 10.2\) Å (droplet 1) and \(\Delta {r}_{{\rm{2}}}=4\sqrt{3}{a}_{0}\approx 17.7\) Å (droplet 2), as shown in the insets of Fig. 4a, b, respectively, where \({a}_{0}=2.55\) Å is the surface nearestneighbor spacing for Cu(111) at 4.2 K. In Fig. 4a, b, we present the experimental \({\mathrm{d}}I/{\mathrm{d}}V\) lineshapes measured via STS at the center and edge sites of these droplets, and for comparison, that of an isolated Co adatom. The \({\mathrm{d}}I/{\mathrm{d}}V\) lineshapes for these two droplets exhibit striking differences: the widths of the Kondo resonances in droplet 2 are significantly enhanced over that of the isolated Co adatom, with the center showing a larger \(\Delta {E}_{{\rm{K}}}\) than the edge site. Using a Fano fit^{28} to extract the width of the Kondo resonance (Supplementary Note 2), and setting \(\Delta {E}_{{\rm{K}}}={k}_{\rm{B}}{T}_{{\rm{K}}}\) (ref. ^{1}), we find that the largest Kondo temperature \({T}_{{\rm{K}}}=72\pm 6\) K is observed at the droplet center, representing an \(\sim {\!\!} 35\)% enhancement over the \({T}_{{\rm{K}}}=53\pm 5\) K of an isolated Co adatom. In stark contrast to this behavior, the corresponding \({\mathrm{d}}I/{\mathrm{d}}V\) lineshapes in droplet 1 are nearly identical to that of an isolated Co adatom, and the widths of their respective Kondo resonances are the same within experimental error. In Fig. 4c, d, we present the theoretically computed \({\mathrm{d}}I/{\mathrm{d}}V\) lineshapes^{24,25,30,31} (see Supplementary Note 4), which well reproduce the experimental results shown in Fig. 4a, b. These results confirm the theoretically predicted enhancement of the width of the Kondo resonance for \(\Delta {r}_{{\rm{2}}}=4\sqrt{3}{a}_{0}\) (see Fig. 3a).
Kondo echo as a signature of quantum coherence
The creation of a coherent Kondo droplet for \(\Delta {r}_{{\rm{2}}}=4\sqrt{3}{a}_{0}\) (droplet 2) leads to another unique effect—the formation of a Kondo echo. When a magnetic adatom is removed from the droplet’s center to create a vacancy, or a Kondo hole (as shown in Fig. 5a, b), the spectral signature of the Kondo effect can be observed nonlocally at this site as a Kondo echo. To demonstrate this, we present in Fig. 5c, d the experimentally measured differential conductance, \({\mathrm{d}}I/{\mathrm{d}}V\), along a line through the center of the uncorrelated Kondo droplet 1 with \(\Delta {r}_{{\rm{1}}}=4{a}_{0}\) and the coherently coupled Kondo droplet 2 with \(\Delta {r}_{{\rm{2}}}=4\sqrt{3}{a}_{0}\) (see horizontal gray lines in Fig. 5e, f), respectively, at \(E=10\) meV, corresponding approximately to the maximal \({\rm{d}}I/{\rm{d}}V\) of the Kondo resonance (see dashed line in Fig. 3b). A comparison of Fig. 5b, d, which both have the same spatial (\(x\)axis) scale, shows that \({\mathrm{d}}I/{\mathrm{d}}V\) exhibits a peak at the sites of each magnetic adatom. Interestingly enough, however, an additional peak in \({\mathrm{d}}I/{\mathrm{d}}V\) – the Kondo echo – occurs at the Kondo hole site in the center of droplet 2. This Kondo signal represents the correlated signature of the Kondo screening cloud of electrons that is macroscopically coherent over the entire droplet. As further evidence of this effect, we show that Kondo droplet 1 (see Fig. 5a), in which the Kondo resonances are essentially decoupled from each other, exhibits no Kondo signal at the center vacancy (see Fig. 5c). Our theoretical results for \({\mathrm{d}}I/{\mathrm{d}}V\) along the same line for the same Kondo droplets with a Kondo hole at the center (see Fig. 5e, f and Supplementary Note 5 for details) very well reproduce these experimental findings (see Fig. 5g, h), and in particular, confirm the existence of a Kondo echo at the vacancy site of Kondo droplet 2 (Fig. 5h), and its absence in droplet 1 (Fig. 5g). The existence or absence of a Kondo echo in droplets 2 and 1, respectively, is further confirmed by the experimentally measured \({\mathrm{d}}I/{\mathrm{d}}V\) lineshape at the center vacancy sites shown in Supplementary Fig. 5 of Supplementary Note 6. While \({\mathrm{d}}I/{\mathrm{d}}V\) at the vacancy site of droplet 2 still exhibits a characteristic Kondo resonance, and hence a Kondo echo, \({\mathrm{d}}I/{\mathrm{d}}V\) at the vacancy site of droplet 1 does not. These results thus demonstrate that the existence of a nonlocal Kondo echo reflects the presence of an extended Kondo cloud that is pervasive and coherent over the entire droplet.
Discussion
The ability to manipulate the strength of Kondo screening, and hence the Kondo temperature, by varying the size, shape, or lattice constant of Kondo droplets opens a venue for the exploration and quantum engineering of manybody effects, and the many ensuing unconventional properties and phases exhibited by strongly correlated electron materials. Future studies will focus on the possibility to tune the competition between Kondo screening and antiferromagnetic correlations – which is at the heart of the heavyfermion problem^{8} – in the same manner as Kondo screening by itself can be manipulated. The creation of Kondo droplets that balance these two competing phenomena such that the addition of a single magnetic adatom could tip the balance one way or another, presents an exciting opportunity to explore this competition. Furthermore, Kondo screening enables the emergence of unconventional superconductivity in many heavyfermion materials, raising the possibility to create superconducting correlations in Kondo droplets, and manipulate the incipient spatial structure of the superconducting order parameter. The recent development of Josephson scanning tunneling spectroscopy^{32,33} would be a suitable tool to probe the emergence of such superconducting correlations on the atomic scale, opening paths for exploring and manipulating not only the emergence of Kondo lattices and heavyfermion physics, but also that of unconventional superconducting phases.
Methods
Theoretical methods
The theoretical results for the local hybridization and Greens functions were obtained using a realspace large\(N\) expansion of the Kondo Hamiltonian (for details see Supplementary Note 1). The differential conductance, \({\mathrm{d}}I/{\mathrm{d}}V\), was computed assuming simultaneous tunneling into the conduction electron and magnetic \(d\)orbitals, with tunneling amplitudes \({t}_{c}\) and \({t}_{f}\), respectively.
Experimental methods and procedures
The single crystal Cu(111) surface was prepared by repeated cycles of Ar+ ion sputtering and annealing in ultrahigh vacuum. After cooling the sample to 4.2 K, an electron beam evaporator was used to dose Co to \(\sim {\!} 4\) atoms/(100 Å)^{2} coverage for the Kondo droplet experiments. The STS tip was then used as an atom manipulator to construct nanoscopic Co lattices comprises 36 Co atoms each of varying geometry. Using scanning tunneling spectroscopy, the differential conductance, \({\mathrm{d}}I/{\mathrm{d}}V\) was measured. Typical spectroscopic measurement parameters: \({R}_{{\rm{T}}}=100\) MΩ –1 GΩ at \(V=10\) mV, \({V}_{\text{ac}}=250\,\)µV – 1 mV rms, \(f{\!}={\!}200\!\!\!1000\) Hz. \({\mathrm{d}}I/{\mathrm{d}}V\) image maps and linecuts were acquired simultaneously with associated topographs by applying an a.c. modulation (typically 250 µV to 1 mV r.m.s. at 201 or 1007 Hz) at a frequency exceeding the bandwidth of the feedback loop, and recording the lockin detected \({\mathrm{d}}I/{\mathrm{d}}V\) (conductance map) along with tip height (topograph) at fixed d.c. bias \(V=10\) mV while the tip was scanned in closedloop constant\(I\) mode. Such scans provided a Kondo signal map proportional to the depletion of the local density of states at \({E}_{\rm{ F}}\) due to the Kondo resonance.
Data availability
The data that support the findings of this study are available from the authors on reasonable request; see author contributions for specific data sets.
Code availability
The codes that were employed in this study are available from the authors on reasonable request.
References
 1.
Manoharan, H. C., Lutz, C. P. & Eigler, D. M. Quantum mirages formed by coherent projection of electronic structure. Nature 403, 512 (2000).
 2.
Moon, C. R., Lutz, C. P. & Manoharan, H. C. Singleatom gating of quantumstate superpositions. Nat. Phys. 4, 454 (2008).
 3.
Hirjibehedin, C. F., Lutz, C. P. & Heinrich, A. J. Spin coupling in engineered atomic structures. Science 312, 1021 (2006).
 4.
Tsukahara, N. et al. Evolution of the Kondo resonance from a single impurity molecule to the twodimensional lattice. Phys. Rev. Lett. 106, 187201 (2011).
 5.
Gomes, K. K., Mar, W., Ko, W., Guinea, F. & Manoharan, H. C. Designer Dirac fermions and topological phases in molecular graphene. Nature 483, 306 (2012).
 6.
Slot, M. R. et al. Experimental realization and characterization of an electronic Lieb lattice. Nat. Phys. 13, 672 (2017).
 7.
Kim, H. et al. Toward tailoring Majorana bound states in artificially constructed magnetic atom chains on elemental superconductors. Sci. Adv. 4, eaar5251 (2018).
 8.
Doniach, S. The Kondo lattice and weak antiferromagnetism. Phys. B 91, 231 (1977).
 9.
von Lohneysen, H., Rosch, A., Vojta, M. & Woelfle, P. Fermiliquid instabilities at magnetic quantum phase transitions. Rev. Mod. Phys. 79, 1015 (2007).
 10.
Gegenwart, P., Si, Q. & Steglich, F. Quantum criticality in heavyfermion metals. Nat. Phys. 4, 186 (2008).
 11.
Scalapino, D. J. A common thread: The pairing interaction for unconventional superconductors. Rev. Mod. Phys. 84, 1383 (2012).
 12.
Stewart, G. R. Unconventional superconductivity. Adv. Phys. 66, 75 (2017).
 13.
Kondo, J. Resistance minimum in dilute magnetic alloys. Prog. Theo. Phys. 32, 37 (1964).
 14.
Wirth, S. & Steglich, F. Exploring heavy fermions from macroscopic to microscopic length scales. Nat. Rev. Mat. 1, 16051 (2016). UNSP.
 15.
Coleman, P. 1/N expansion for the Kondo lattice. Phys. Rev. 28, 5255 (1983).
 16.
Hewson, A. C. The Kondo Problem to Heavy Fermions. (Cambridge University Press, Cambridge, England, 1993).
 17.
Senthil, T., Vojta, M. & Sachdev, S. Weak magnetism and nonFermi liquids near heavyfermion critical points. Phys. Rev. B 69, 035111 (2004).
 18.
Si, Q., Rabello, A., Ingersent, K. & Lleweilun Smith, J. Local fluctuations in quantum critical metals. Phys. Rev. B 68, 115103 (2003).
 19.
Ohashi, T., Suga, S. & Kawakami, N. Magnetic properties of a Kondo insulator with RKKY interaction: extended dynamical mean field study. J. Phys.: Condens. Matter 17, 4547 (2005).
 20.
Paul, I., Pepin, C. & Norman, M. R. Kondo breakdown and hybridization fluctuations in the KondoHeisenberg lattice. Phys. Rev. Lett. 98, 026402 (2007).
 21.
Read, N. & Newns, D. M. On the solution of the CoqblinSchrieffer Hamiltonian by the largeN expansion technique. J. Phys. C. 16, 3273 (1983).
 22.
Bickers, N. E. Review of techniques in the largeN expansion for dilute magnetic alloys. Rev. Mod. Phys. 59, 845 (1987).
 23.
Affleck, I. & Marston, B. Largen limit of the HeisenbergHubbard model: implication for high\({T}_{c}\) superconductors. Phys. Rev. B 37, 3774 (1988).
 24.
Figgins, J. & Morr, D. K. Differential conductance and quantum interference in kondo systems. Phys. Rev. Lett. 104, 187202 (2010).
 25.
Morr, D. K. Theory of scanning tunneling spectroscopy: from Kondo impurities to heavy fermion materials. Rep. Prog. Phys. 80, 014502 (2017).
 26.
Simon, E. et al. Exchange interaction between magnetic adatoms on surfaces of noble metals. Phys. Rev. B 83, 224416 (2011).
 27.
Chen, W., Jamneala, T., Madhavan, V. & Crommie, M. F. Disappearance of the Kondo resonance for atomically fabricated cobalt dimers. Phys. Rev. B 60, R8529 (1999).
 28.
Fano, U. Effects of configuration interaction on intensities and phase shifts. Phys. Rev. 124, 1866 (1961).
 29.
Raczkowski, M. & Assaad, F. F. Emergent coherent lattice behavior in Kondo nanosystems. Phys. Rev. Lett. 122, 097203 (2019).
 30.
Maltseva, M., Dzero, M. & Coleman, P. Electron cotunneling into a Kondo lattice. Phys. Rev. Lett. 103, 206402 (2009).
 31.
Wölfle, P., Dubi, Y. & Balatsky, A. V. Tunneling into clean heavy fermion compounds: origin of the fano line shape. Phys. Rev. Lett. 105, 246401 (2010).
 32.
Hamidian, M. H. et al. Detection of a cooperpair density wave in Bi\({}_{2}\)Sr\({}_{2}\)CaCu\({}_{2}\)O\({}_{8+x}\). Nature 532, 343 (2016).
 33.
Graham, M. & Morr, D. K. Josephson scanning tunneling spectroscopy in \({d}_{{x}^{2}{y}^{2}}\)wave superconductors: A probe for the nature of the pseudogap in the cuprate superconductors. Phys. Rev. Lett. 123, 017001 (2019).
Acknowledgements
This work was supported by the U. S. Department of Energy, Office of Science, Basic Energy Sciences, under Award No. DEFG0205ER46225 (J.F., D.K.M.), and by the Department of Energy, Office of Science, Basic Energy Sciences, Materials Sciences and Engineering Division, under Contract DEAC0276SF00515 (L.S.M., W.M., Y.T.C., H.C.M.).
Author information
Affiliations
Contributions
D.K.M. and H.C.M. devised the project and wrote the manuscript. J.F. and D.K.M. conducted the theoretical calculations. L.S.M, W.M, Y.T.C. and H.C.M. performed experiments and data analysis.
Corresponding authors
Correspondence to Hari C. Manoharan or Dirk K. Morr.
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Peer review information Nature Communications thanks Markus Ternes and the other, anonymous, reviewer(s) for their contribution to the peer review of this work.
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Figgins, J., Mattos, L.S., Mar, W. et al. Quantum engineered Kondo lattices. Nat Commun 10, 5588 (2019). https://doi.org/10.1038/s41467019134461
Received:
Accepted:
Published:
Further reading

Creating designer quantum states of matter atombyatom
Nature Reviews Physics (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.